Assembly of niobium-phosphate cluster and in-situ transition-metal-containing derivatives
Zhao, Shufang; Liang, Zhijie; Geng, Qiaohua; Ma, Pengtao; Zhang, Chao; Niu, Jingyang; Wang, Jingping; CrystEngComm  (2017) –; doi:10.1039/C7CE00603A

data_7228092
_publ_section_title
;
 Assembly of niobium-phosphate cluster and in-situ
 transition-metal-containing derivatives
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/C7CE00603A
_journal_year                    2017
_chemical_formula_moiety         '0.5(Cs6 Nb12 O95 P8 Zn4), 2(O)'
_chemical_formula_sum            'Cs3 H28 Nb6 O50 P4 Zn2'
_chemical_formula_weight         2039.03
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_primary     direct
_audit_creation_date             2017-03-25
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_audit_update_record
;
2017-03-27 deposited with the CCDC.
2017-04-19 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 109.375(5)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.558(4)
_cell_length_b                   20.153(7)
_cell_length_c                   10.614(4)
_cell_measurement_reflns_used    6922
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.33
_cell_measurement_theta_min      2.87
_cell_volume                     2130.5(14)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL-2014/7 (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296.15
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0213
_diffrn_reflns_av_unetI/netI     0.0235
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            10850
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.100
_diffrn_reflns_theta_max         25.100
_diffrn_reflns_theta_min         2.021
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    5.475
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4623
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2008/1 (Bruker,2008) was used for absorption correction.
wR2(int) was 0.1306 before and 0.0365 after correction.
The Ratio of minimum to maximum transmission is 0.6200.
The \l/2 correction factor is 0.0015.
;
_exptl_crystal_colour            yellow
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    3.179
_exptl_crystal_description       block
_exptl_crystal_F_000             1918
_exptl_crystal_size_max          0.39
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.016
_refine_diff_density_max         3.593
_refine_diff_density_min         -2.722
_refine_diff_density_rms         0.230
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.035
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     308
_refine_ls_number_reflns         3782
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0609
_refine_ls_R_factor_gt           0.0558
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0801P)^2^+38.7921P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1476
_refine_ls_wR_factor_ref         0.1528
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3418
_reflns_number_total             3782
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7ce00603a2.cif
_cod_data_source_block           njy1
_cod_original_cell_volume        2130.4(12)
_cod_database_code               7228092
_shelx_estimated_absorpt_t_max   0.918
_shelx_estimated_absorpt_t_min   0.224
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O5W) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
2. Others
 Fixed Sof: Cs1(0.9) Cs1'(0.1) Cs2(0.5) O5W(0.5) O8W(0.25)
;
_shelx_shelxl_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'